



@article {2624,
	title = {Reinforcement of hydroxyapatite by adding P                    2O
                    5-CaO glasses with Na
                    2O, K
                    2O and MgO
},
	journal = {Journal of Materials Science: Materials in MedicineJ. MATER. SCI. MATER. MED.},
	volume = {7},
	year = {1996},
	note = {Cited By (since 1996): 49Export Date: 21 November 2012Source: ScopusCODEN: JSMMELanguage of Original Document: EnglishCorrespondence Address: Santos, J.D.; Dept. of Metallurgical Engineering, FEUP, University of Porto, Rua dos Bragas, 4099 Porto Codex, PortugalChemicals/CAS: hydroxyapatite, 1306-06-5, 51198-94-8; magnesium oxide, 1309-48-4, 1317-74-4References: Barney, V.C., Levin, M.P., Adams, D.F., (1986) J. Perio Dont., 57, p. 764;Legeros, R.Z., (1988) Adv. Dent. Res., 2, p. 164; 
Aoki, H., (1991) Science and Medical Applications of Hydroxyapatite, p. 165. , Takayama Press System Center, JAAS, Tokyo; 
Ducheyne, P., (1987) J. Biomed. Mater. Res. Appl. Biomater., 21, p. 219; 
Heughbaert, J.C., Bonel, G., (1986) Biological and Biomechanical Performance of Biomaterials, p. 9. , edited by P. Christel, A. Meunier and A. J. C. Lee Elsevier Science Publishers B.V., Amsterdam; 
Ellis, L.G., Nelson, D.G.A., Featherstone, J.D.B., (1988) J. Biomed. Mater. Res., 22, p. 541; 
Raemdonck, W.V., Ducheyne, P., Meester, P.D., (1984) Metal and Ceramic Biomaterials, p. 143. , edited by P. Ducheyne and G. W. Hashi CRC Press, Boca Raton, FL; 
Shors, E.C., Holmes, R.E., (1993) An Introduction to Bioceramics, p. 181. , edited by L. L. Hench and J. Wilson World Scientific, Hong Kong; 
Rey, C., (1990) Biomaterials, 11, p. 14; 
Evans, G., Behiri, J., Currey, J., Bonfield, W., (1990) J. Mater. Sci. Mater. Med., 1, p. 38; 
Rey, C., Fr{\`e}che, M., Heughebaert, M., Heughebaert, J.C., Lacout, J.L., Vignoles, M., Bioceramics 4, London, 1991, p. 57. , edited by W. Bonfield, G. W. Hastings and K. E. Tanner (Butterworth-Heinemann, London); 
With, G., Van Dijk, H., Hattu, N., Prijs, K., (1981) J. Mater. Sci., 16, p. 1592; 
Akao, M., Aoki, H., Kato, K., (1981) J. Mater. Sci., 16, p. 809; 
Santos, J., Knowles, J., Reis, R., Monteiro, F., Hastings, G., (1994) Biomaterials, 15, p. 5; 
Soltesz, U., Richter, H., Kienzler, R., (1987) High Technology Ceramics, p. 110. , Elsevier Science Publishers, B.V., Amsterdam; 
(1971) Determination Micrographique de la Grosseur du Grain Ferritique ou Aust{\'e}nitique des Aciers; 
Daculsi, G., LeGeros, R.G., Nery, E., Lynch, K., Kerebel, B., (1989) J. Biomed. Mater. Res., 23, p. 883
},
	month = {1996///},
	pages = {187 - 189},
	publisher = {Chapman \& Hall Ltd},
	abstract = {Commercial hydroxyapatite was reinforced by adding small amounts (2 and 4 wt\%) of P                        2O
                        5-based glasses during its sintering process. The composites prepared had a chemical composition closely related to the mineral part of bone tissues in terms of trace elements usually detected, such as Na, K and Mg. X-ray diffraction analysis (XRD) showed that the glass reinforced-HA composites were composed of a HA matrix and variable amounts of tricalcium phosphate phase, depending on sintering temperature and glass composition. These composites were shown to have much higher biaxial bending strength than sintered HA, 107 MPa for Ha/2\% of 35P
                        2O
                        5-35CAO-10Na
                        2O-10K
                        2O-10MgO glass composite and 28 MPa for sintered HA. The presence of β-tricalcium phosphate in the microstructure of the composites is an important factor in the reinforcement process.
Commercial hydroxyapatite was reinforced by adding small amounts (2 and 4 wt\%) of P
                        2O
                        5-based glasses during its sintering process. The composites prepared had a chemical composition closely related to the mineral part of bone tissues in terms of trace elements usually detected, such as Na, K and Mg. X-ray diffraction analysis (XRD) showed that the glass reinforced-HA composites were composed of a HA matrix and variable amounts of tricalcium phosphate phase, depending on sintering temperature and glass composition. These composites were shown to have much higher biaxial bending strength than sintered HA, 107 MPa for Ha/2\% of 35P
                        2O
                        5-35CaO-10Na
                        2O-10K
                        2O-10MgO glass composite and 28 MPa for sintered HA. The presence of β-tricalcium phosphate in the microstructure of the composites is an important factor in the reinforcement process.
},
	keywords = {article, Bending strength, Bone, chemical composition, Composite materials, Composition, Composition effects, glass, Glass composition, Glass reinforced hydroxapatite composite, hydroxyapatite, implant, Magnesium Oxide, metal oxide, Microstructure, molecular dynamics, Phosphates, potassium derivative, priority journal, Sintering, Sintering temperature, sodium derivative, Thermal effects, Trace Elements, Tricalcium phosphate phase, X ray diffraction},
	isbn = {09574530 (ISSN)},
	url = {http://www.scopus.com/inward/record.url?eid=2-s2.0-0030108677\&partnerID=40\&md5=e9c978c3e018a1dd2db9b534ef00ea1b},
	author = {Santos, J.D. and Silva, P.L. and Knowles, J.C. and Talal, S. and Monteiro, F.J.}
}
